Upload
others
View
8
Download
0
Embed Size (px)
Citation preview
Cladding Process Simulation And Residual Stress Estimation Using Finite Element Coupled
Field Analysis
GK Purohit1, Kalakesh Baligar2 1Professor, Mechanical Engineering Department, PDA College of Engineering, Gulbarga, Karnataka, India
2MTech (Production Engineering) Student, PDA College of Engineering, Gulbarga, Karnataka, India
Abstract Material properties like hardness, yield strength,
corrosion resistance, conduction properties plays important
role in structural design and product life cycle. It is difficult
to get a material with all required properties. So cladding is
done to improve the required properties on the surface of the
base metal. A number of experimental methods are there to
determine the residual stresses produced during welding.
However, a Finite element analysis is found to yield better
approximations and also to analyze the thermo structural
behavior of cladding process. Hence, in the present work an
attempt is made to employ the Finite Element Analysis for the
same. SA508 material is considered as the base material and
cladding materials are changed to predict the nature of
residual stresses. Element birth and death feature of ANSYS
software is used to simulate the cladding process. Initially
the geometry is built using top down approach of ANSYS.
The geometry is split to ease the brick meshing of the
geometry. With the appropriate elements, initially thermal
analysis is carried out to find temperature distribution
during cladding process. Block by block cladding simulation
is carried out. Finally the structure is cooled it its initial
temperature (No load condition) and coupled field analysis is
carried out to find the residual stress nature. The effects of
thickness on nature of residual stresses are also analyzed.
Further analysis is carried out with general clad materials
(Aluminium, brass and Zirconium).
.
Keywords––ANSYS, Submerged Arc Welding, Strip
Cladding, Residual Stresses, Finite Element Analysis.
1. Introduction
1.1 Introduction
Materials nowadays require multiple conflicting
properties such as high hardness and ductility. Different
properties however are often required at different locations
on the products. Wear and corrosion resistance are only
required at the surfaces of products for instance. Surfaces of
materials are always in contact with their surrounding,
resulting in degradations due to wear, erosion and corrosion.
Surface modification aims at reducing such surface
degeneration. Surface modification may involve the
application of a coating, for instance by using chemical
vapour deposition, plasma spraying and strip cladding.
Surface modification can be applied to all kinds of products
to increase performance, reduce costs, and modify the
surface properties independent of the bulk material. This
enables the realization of products with improved
functionality, at reduced use of scarce and expensive
materials.
1.2 Cladding:
Cladding is a process where one material covers
another. Cladding supplies a combination of desired
properties not found in any one metal. A base metal can be
selected for cost or structural properties, and another metal
added for surface protection or some special property such as
electrical conductivity. Thickness of the cladding can be
made much heavier and more durable than obtainable by
electroplating.
1.2.1 Strip Cladding
A superior coating technique, which manifests a
metallic bonding of substrate and coating, is the Strip
cladding technique. Strip cladding has become an important
surface modification technique in today’s industry and
continues to gain market. Strip cladding is not only applied
for coating but also for repair and refurbishment as well as
for rapid prototyping.
Fig. 1.1: Submerged Arc Strip Cladding
There are two types of Strip Cladding processes.
1) Submerged Arc Strip Cladding 2) Electro Slag Strip
Cladding
Submerged Arc Strip Cladding utilizes an arc that
runs back and forth at high speed along the strip, depositing
weld metal onto the base material. Because this is an arc
process there will be penetration into the base material
resulting in dilution levels of 20%. Deposition rates are in the
region of 10/12kg/hr for 60mm strip and are restricted by
how much current can be applied.
Electro Slag Strip Cladding (ESW) utilizes a
conductive flux and the resulting Joule heating effect to melt
the strip into the liquid slag; which is transferred into molten
metal deposited onto the base material. Higher current levels
can be used giving deposition rates of 22-25kg/hr for 60mm
strip.(SAW 10/12kg/hr). Utilizing high speed fluxes, dilution
levels can be reduced and the area coverage (M2/hr) can be
increased.
1.2.2 SAW cladding
SAW can be applied for joining and for overlay
welding, i.e. depositing a corrosion resistant layer onto a
mild (carbon) or low-alloyed steel. SAW produces
coalescence of metals by heating them with an arc between a
bare metal electrode and the work. The arc and molten metal
are”submerged” in a blanket of granular fusible flux on the
work piece. This flux plays a main role in that (i) the stability
of the arc is dependent on the flux, (ii) mechanical and
chemical properties of the final weld deposit can be
controlled by the flux, and (iii) the quality of the weld may
be affected by the care and handling of the flux. The flux
also protects the welder from fumes and radiation, which
raise environment advantages. The SAW process can only be
used in a flat position (deviations of up to 6-8° may be
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
1www.ijert.org
IJERT
possible) since it would be difficult to retain the flux and
steel melt in the inclined position. The wire (or strip)
electrode is inserted into a mould of flux that covers the area
or joint to be welded. An arc is initiated and a wire-feeding
mechanism then begins to feed the electrode towards the
joint at a controlled rate. Additional flux is continuously fed
in front and around the electrode, and continuously
distributed over the joint. Heat evolved by the electric arc
progressively melts some of the flux, the end of the
electrode, and the adjacent edges of the base metal, creating a
pool of molten metal beneath a layer of molten slag. The
melted slag bath near the arc is in a high turbulent state. Gas
bubbles are quickly swept to the surface of the pool. As the
welding zone progresses along the seam, the weld metal and
then the liquid flux cool and solidify, forming a weld bead
and a protective slag shield over it. Welding electrodes are
supplied as solid wire, metal cored wire or strips. The
electrodes can have a thin copper coating to provide good
electrical contact, except those for welding corrosion
resisting materials or for certain nuclear applications. Wire
electrodes vary in size from 1.6 to 6 mm in diameter. The
thickness of strips can vary between 0.5 to 1 mm and the
width between 25 to 200 mm. A commonly used size is 60 x
0.5 mm. The main object of the flux is to protect the arc and
weld pool from contamination with atmospheric oxygen and
nitrogen. The flux should also provide arc stabilization
properties, i.e. to facilitate ionization of the arc column. In
addition the flux, when melted, should also provide slag of
suitable viscosity and surface tension to ensure welds of
good surface finish and shape.
Fig. 1.2: Principle of SAW welding
Parameters of cladding quality:
a) Welding current
The strip cladding process is almost always
performed with the positive polarity on the strip electrode
(DCEP). With negative polarity, there is less penetration, and
the weld bead tends to be thicker which could give steeper
bead edges with increased risk for welding defects in the
overlapping zones. The current transfer across the arc is not
uniform across the width strip, as there is not one but a series
of small arcs that wander across the end of the strip in the
melting zone. A typical current density for SAW strip
cladding is within the range 20 to 25A/mm2. Increasing the
current level will lead to a higher deposition rate but also the
dilution will be higher.
b) Welding voltage
The optimum arc voltage to be used depends on
different factors such as the welding flux, welding position
and welding current. Increasing the voltage will lead to an
increase in flux consumption.
c) Travelling speed
The welding travelling speed is generally related to
the welding current being used and these two parameters are
adjusted in tandem to give the desired combination of bead
profile and bead thickness. Increasing the welding speed will
lead to an increase of dilution.
Advantage of SAW
High deposition rates(45kg/h) have been reported
High operating factors in mechanized applications
Deep weld penetration
High speed welding of thin sheet steels upto 5m/mm is
possible
Minimal welding fume or arc light is emitted
Distortion is much less
Welds produced are sound, uniform, ductile and
corrosion resistant and have good impact value
50 to 90% of flux is recoverable
Limitations of SAW:
Limited to ferrous(steel or stainless steels) and some
nickel based alloys
Normally limited to long straight seams or rotated pipes
or vessels.
Requires relatively troublesome flux handling systems
Flux and slag residue can present a health & safety
concern.
Requires inter-pass and post weld slag removal.
Applications of SAW:
SAW is used for welding low carbon and medium
carbon steel.
For welding stainless steels, copper, aluminium and
titanium base alloys
SAW is also capable of welding heat resistant steels,
corrosion resistant steels and high strength steels.
SAW is widely used for butt and fillet welds in heavy
industries like shipbuilding, pressure vessel fabrication,
rail road tank cars, structural engineering, pipe welding
and for storage tanks.
Thinner material products such as water heaters and
propane tanks.
Hard facing for steel mills, earthmoving equipment,
mining etc.
1.3 Cladding residual stresses
Because of significant difference in the thermal
expansion coefficient between the austenitic cladding and the
ferritic base metal, thermal stresses are induced in the
cladding and the underlying base metal. Even after stress
relieving and cooling down to room temperature, stresses of
yield magnitude can be induced in the cladding and the
cladding HAZ. The cladding residual stresses are
temperature dependent, and decrease as the temperature
increases. The magnitude and distribution of the cladding
residual stresses depend on the temperature history during
the cladding procedure, the geometry of the cladded
component, the thickness of the cladding, the material
properties of the base metal and the cladding, and the heat
and pressure treatments both before and after the cladding
process. These residual stresses are complex and often
evaluated with the aid of experiments combined with
computational modelling. Several destructive and non
destructive methods are available for measurement of
residual stresses; each having its advantages and
disadvantages. Experimental evaluations are often based on
laboratory tests conducted with specimens that are machined
from cladded components. The experimental methods for
determining the through-thickness residual stresses are based
on relaxation technique and are destructive procedures, since
they require cutting and machining of the plate.
Deformations resulting from each cutting and machining step
are monitored by surface strain gauges. These deformations
are input data in a computational procedure which calculates
the residual stresses that existed in the cladded plate before
cutting. However, due to the differences in geometric
stiffness (degree of restraint) in a laboratory small specimen
and a real large structure, the experimental results from a
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
2www.ijert.org
IJERT
small specimen should be corrected to correspond to the real
situations in the structure (reactor pressure vessel). This point
has normally been ignored in the studies reported in the
literature. Numerical evaluations of cladding residual stresses
are often based on finite element analyses. However, there
are many temperature dependent parameters which affect the
magnitude and distribution of cladding residual stresses, and
computational analyses are therefore normally performed
under certain simplified assumptions.
2. Literature Survey
Literature survey on residual stresses:
A comprehensive literature search revealed a
number of previous works on the subject of residual stress
(R.S.) analysis. Heyn and Bauer [1], in their research on
residual stresses in cold-drawn metals, illustrated the spring
analogy to show how the residual stresses in metals behave.
The amount of elongation experienced by the center springs
is directly proportional to the force exerted on them by the
outer springs. An exact method of determining the
longitudinal, tangential, and radial residual stresses in bars or
tubes was proposed by Mesnager [2] and modified by
Sachs[3]. The method is limited to cylindrical bodies in
which the residual stresses vary in the radial direction but are
constant in the longitudinal and circumferential directions.
The reaction of a material to externally applied stresses is
influenced by the presence of residual stresses. On the other
hand, compressive residual stresses will increase the yield
stress. This principle first was employed in 1888 to
manufacture built-up guns Hayes[4]. Timoshenko[5]
presented a review of the early literature and theoretical
treatment of manufactured parts such as guns and turbine
rotors. Robertson[6] stated that residual stresses are as
effective as stresses due to externally applied loads in
producing stress corrosion cracking. A study was made by
Demorest[7] of electro polishing methods of the residual
stresses imposed upon copper strips subjected to various
degrees of cold drawing and cold rolling. Analysis was made
from the nature of the equilibrium distribution, which was
determined experimentally by observing the curvature
changes that occurred as thin layers of surface material were
stripped. Horger[8] (1948) claimed that residual stresses in
an elastic member would arise from three distinct sources
namely misfit, change in specific volume, and non-uniform
distortion. In a paper published by Leeser and Daane[9], the
electro-polishing techniques were presented in a relatively
simple and accurate way to determine residual stresses in a
strip of rectangular cross section in terms of strain changes
during electro-polishing. Dieter[10] stated that residual
stresses cannot be determined directly from strain-gauge
measurements, as is the case for stresses due to externally
applied loads. Rather, residual stresses are calculated from
the measurements of strain that are obtained when the body
is sectioned and the locked-in residual stresses are released.
Srinivasan, Hartley and Bandy[12] showed that
electrochemical machining (ECM) provides a rapid, easily
controlled and damage-free method of metal removal. P.
Dupas[18] in his article “Evaluation of Cladding Residual
Stresses in Clad Blocks by Measurements and Numerical
Simulations” discussed about cladding process in the reactor
vessels and measurement of residual stresses”. According to
these measurements, transversal stresses (perpendicular to
the welding direction) and longitudinal stresses (parallel to
the welding direction) are highly tensile in stainless steel and
they are compressive in the HAZ. Finite element calculations
were used to simulate both welding operations and post weld
heat treatment. These calculations coupled the thermal,
metallurgical and mechanical aspects in a 2D representation.
Different models were studied including effect of generalized
plane strain, transformation plasticity, creep and tempering.
The transversal stresses calculated are similar to the
measured ones, but the longitudinal stresses showed to be
very sensitive to the model used.
1.4.2. Literature Survey on Thermal Stresses
I. J. Kumar, D. Rajgopalan [11] presented Steady
state thermal analysis and deformations in a hollow circular
cylinder being head at the internal surface by a source which
is sinusoidal along the length of the cylinder and with
Newton type radiation boundary condition at the outer
surface. The solution of the problem under given boundary
condition has been obtained in the form of infinite integrals.
G. Sánchez Sarmiento, M.J. Mizdrahi, P. Bastias and M.
Pizzi [19] reviewed several finite element models for the
determination of mechanical and thermal stresses in the SHS
(Secondary Heat Sink) System. The models were developed
by ABAQUS/CAE, solving with ABAQUS/Standard the
problems of temperature distribution and of thermo-elastic-
plastic stress and strain distribution of several components,
subjected to complex loads of normal operation as well as
postulated accidents. The design was based on internal
pressure load, and further analysis take into account thermal
shock, thermal stratification and pipe forces. Muhammad
Abid [20] carried out analysis to investigate joint strength
and sealing capability under combined internal pressure and
different steady-state thermal loading, a 3D nonlinear finite
element analysis (FEA) of a gasketed flange joint is carried
out and its behaviour is discussed. They concluded that at
higher temperatures the internal pressure must be lower for
safe operating conditions.
M. Murali Krishna, M.S. Shunmugam and N. Siva Prasad
[21] presented a three-dimensional finite element analysis
(FEA) of bolted flange joints carried out by taking
experimentally obtained loading and unloading
characteristics of the gaskets. Experiments have been carried
out for finding the loading and unloading characteristics of
the gasket materials, which are in turn used in the FEA. The
increase in the axial bolt force when the joint is subjected to
an internal pressure has also been analyzed. Analysis shows
that the distribution of contact stress has a more dominant
effect on sealing performance than the limit on flange
rotation specified by ASME. Mohammad A. Irfan and Walter
Chapman [24] performed analysis of the thermal stresses in
radiant tubes. The analytical analysis is verified using a finite
element model. It was found that axial temperature gradients
are not a source of thermal stresses as long as the
temperature distribution is linear. Symmetric circumferential
gradients generate thermal stresses, which are low as
compared to the stress rupture value of radiant tubes. Radial
temperature gradients create bi-axial stresses and can be a
major source of thermal stress in radiant tubes. They
concluded that the bends carry a higher stress level than the
straight portion of the tube and a local hot spot generates
stresses, which can lead to failure of the tube.
3. Problem Definition & Scope of the Work
3.1 Definition
“Evaluation of Residual Stresses in Clad Blocks
and the base metal by Numerical Simulations is the main
objective of the problem. So the problem objectives include:
Finite element modelling of cladding process
Finding temperature distribution across the base metal
and clad metal
Finding residual stresses in the cladding process
Effect of thickness of cladding layer in residual stress
formation
Effect of material properties on residual stress
formation
Results presentation
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
3www.ijert.org
IJERT
3.2 Methodology
Geometrical modelling of the clad material with the
parent material using ANSYS top-down approach
Brick-meshing of both parent and clad material
Application of initial thermal boundary conditions
Analysis for thermal results
Coupled field analysis to find the residual stresses in the
structure
Representation of the graphical plots
Results representation for variation in parameters
Graphical plots for both temperature and stress across
the thickness direction.
Report generation
3.2.1 Flow chart for thermal analysis using ANSYS
ANSYS is a suite of powerful engineering
simulation programs, based on the finite element method that
can solve problems ranging from relatively simple linear
analyses to the most challenging nonlinear simulations.
ANSYS contains an extensive library of elements that can
model virtually any geometry. Designed as a general-purpose
simulation tool, ANSYS can be used to study more than just
structural (stress/displacement) problems. It can simulate
problems in such diverse areas as heat transfer, mass
diffusion, thermal management of electrical components
(coupled thermal-electrical analyses), acoustics, soil
mechanics (coupled pore fluid-stress analyses), and
piezoelectric analysis. In most simulations, including highly
nonlinear ones, the user need only provide the engineering
data such as the geometry of the structure, its material
behavior, its boundary conditions, and the loads applied to it.
In a nonlinear analysis ANSYS automatically chooses
appropriate load increments and convergence tolerance.
Fig. 3.1: Flow chart for ANSYS thermal analysis
3.2.2 ANSYS structural analysis from thermal results Thermal results are taken to structural analysis as
shown in the following block diagram (Fig. 3.2) for stress
and deformation results.
Fig. 3.2: Block Diagram of thermal structural analysis
The basic procedure for sequential coupled field
thermal structural analysis is as given below.
Define the thermal problem.
Write the thermal file.
Clear boundary conditions and options.
Define the structural problem.
Write the structural file.
Read the thermal file.
Solve and postprocessor the thermal problem.
Read the structural file.
Read the temperatures from the thermal results file.
Solve and postprocessor the file.
3.3 Material Properties
Table 3.1: Material Properties
Property Value
Base Metal : Ferritic
steel (SA508)
Young’s Modulus 206GPa
Poison’s ratio 0.3
Density 7800Kg/m3
Thermal Conductivity 42w/m –K
Specific heat 365W
Thermal expansion
Coefficient
11.7/0c
SA304
Young’s Modulus 196GPa
Poison’s ratio 0.3
Density 7800Kg/m3
Thermal Conductivity 15w/m –K
Specific heat 465W
Thermal expansion
Coefficient
18.7/0c
3.4 Initial Geometrical Model:
Fig. 3.3: Geometrical Model of the problem
The figure 3.3 shows geometrical model of the
base metal and clad material. The geometry is built using
Ansys top down approach. The clad blocks are split and
glued to the parent metal brick meshing. Ansys sweep
mesher can brick mesh glued regular structures. Total 10
clad blocks are used for geometrical representation. 200mm
length with 50mm depth is considered for the base metal.
20mm length by 10mm thickness is considered for the clad
material. Due to dynamic nature of the structure the
modelling is carried out in meters.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
4www.ijert.org
IJERT
Fig. 3.4: Meshed Model
Fig. 3.5: Zoomed view of the Mesh
The figure shows brick mesh of both clad material
and base material. Total numbers of elements are 4200 and
numbers of nodes are 19393 nodes. Solid90 element
properties are applied for the structure. For structural
analysis, solid 95 element properties are applied on the
process. Element birth and death property is used to simulate
the process of cladding. The boundary conditions are
changed as per the application of cladding process and
continued till the complete process is done. Different colours
show application of different material properties to the clad
material and to the base metal. Initial complete geometry is
meshed, but boundary conditions are applied only to the
required geometry by killing unnecessary elements. Newton
Raphson solver allows the execution of this type of
problems.
The cladding region is fine meshed to obtain better
results due to higher variation across the thickness of the
structure and due to nearness of the metal to heat conditions.
10 elements are considered across the thickness of 4mm with
0.4mm size for the height along the height of the structure.
3.5 Element:
SOLID90 has a 3-D thermal conduction capability.
The element has eight nodes with a single degree of freedom,
temperature, at each node. The element is applicable to a 3-
D, steady-state or transient thermal analysis. The element
also can compensate for mass transport heat flow from a
constant velocity field. If the model containing the
conducting solid element is also to be analyzed structurally,
the element should be replaced by an equivalent structural
element
Fig. 3.6: Solid70 Element
3.6 Assumptions:
The material is assumed to be in homogenous.
20 noded brick element is used for analysis
All approximations applied to FEM are applicable for
the analysis(FEM is approximate technique)
ANSYS coupled field analysis used for structural and
thermal results
Residual stresses obtained after cooling it to room
temperature
IV. RESULTS & DISCUSSION Analysis has been carried out to find temperature
distribution and residual stresses due to cladding by element
birth and death feature. The bottom of the base material is
insulated for thermal boundary conditions and convection
loads are applied on the top. The initially the body is heated
to 170 0c. The results are as follows.
4.1 Cladding Simulation with Steel
Fig. 4.1: Initial Condition of the problem
Fig 4.2: Temperature distribution in the member
The figure 4.1 shows initial boundary conditions
applied on the problem. A uniform temperature of 1700 is
applied on the geometry. This was taken as the initial step
for transient thermal analysis. Since no cladding process is
started, no clad elements can be observed.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
5www.ijert.org
IJERT
The figure 4.2 shows temperature distribution in
the member. Maximum temperature is around 1700 and
minimum is 170°C. By using element birth and death
properties, elements which are subjected to cladding are
made visible. Other elements are killed and hidden from the
visibility. Maximum temperature can be observed at the top
and reducing towards the base metal. At the base of base
material, almost a temperature of 170°C can be observed.
Away from the cladding region, the temperatures are
minimum. A step size of 0.5 second is used to reduce the
computational times.
Fig. 4.3: Temperature across the thickness of the overall
assembly
Fig. 4.4: Temperature distribution
The temperature is plotted from the top clad
surface to the base material. The graph shows parabolic drop
of temperature from top to bottom. Maximum temperatures
are observed at the top and minimum at the base. The
distance is represented in meters.
The figure shows temperature distribution in the
member. Maximum temperature is around 1700°C and
minimum is 170°C. By using element birth and death
properties, elements which are subjected to cladding are
made visible. Other elements are killed and hidden from the
visibility. Now two clad blocks are visible and maximum
temperature is observed at the present clad block and
temperature is dropped at the previous clad block. The status
bar at the bottom shows variation of temperature with colour
code. Also not much heat is transferred
Fig. 4.5: Cladding at 3 block
Fig. 4.6: Cladding at 4 block
Fig. 4.7: Cladding at 5 block
Fig. 4.8: Cladding at 6 block
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
6www.ijert.org
IJERT
Fig. 4.9: Cladding at 7 block
Fig. 4.10: Cladding at 8 block
Fig. 4.11: Cladding at 9 block
Fig. 4.12: Cladding at 10 block
The temperature distribution after one cycle of
cladding is over. Minimum temperature of around 251.65 0c can be observed by the end of cladding process at the start
of cladding. Maximum temperatures are concentrated
around the cladding region. Totally 40 steps are considered
with each time step of 4seconds with sub step size of 0.5
seconds.
Fig. 4.13: Temperature variation the end of the cladding
process
Fig. 4.14: After 2000 seconds cooling
The graph shows variation of temperature across
the clad region along the thickness direction. The drop of
temperature is parabolic from top to bottom. Minimum
temperatures are shows at the bottom and maximum at the
top surface or cladding region. The X-axis is represented
with distance measured in meters from top clad surface to
bottom base metal.
The figure 4.14 shows temperature variation in the
problem after cooling it for 2000 seconds to the base
temperature. Maximum temperature can be observed at the
base as this region is insulated from heat transfer. The
temperatures in the other regions are represented with
various colours.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
7www.ijert.org
IJERT
Fig. 4.15: After cooling temperature distribution in the
structure
After cooling to the initial temperature,
temperature plot is done to check the distribution. Almost,
the same temperature can be observed across the geometry.
Both clad material and base materials are brought to the
initial temperature. At this point analysis is changed to
Structural analysis from thermal loads. Bottom is
constrained in all directions and thermal loads are taken from
the thermal analysis to the corresponding nodes. The element
type is switched from thermal element Solid90 to 20 noded
structural element Solid95. The analysis is purely carried out
only for thermal loads.
Fig. 4.16: Overall Stress in the structure
Fig 4.17: Base Metal Stress
The figure 4.16 shows vonmises stress in the
structure. The bottom is observed more stress compared to
the top region. Uniform stress variation can be observed
from the top to the bottom geometry. Almost a stress of 38.2
Mpa can be observed at the interface between clad material
and the base material. Also boundary conditions plays
important role in the stress generation, as they allow free
expansion which induce no stress in the structure.
The figure 4.17 shows stress generation in the base
material. Minimum stress is observed on the top surface and
maximum stress in the constrained region. This can be
attributed to cantilever type arrangement due to higher
deflection at the top which results in higher stress generation
at the fixed ends.
Fig 4.18: Stress in the Base Metal (from the top surface)
Fig. 4.19: Stress graph across the clad material
The figure 4.18 shows stress variation in the base
material from top to the fixed end. Slightly higher stress can
be observed at the interface and dropping to the initial depth.
Later stress is increasing to the fixed region. Maximum
stress is observed at the fixed region. A path is defined
across the geometry from top to bottom of the structure by
selecting the nodes and stress is mapped to obtain the graph.
The figure 4.19 shows residual stress generation in
the clad material. Maximum stress observed at the center of
the clad material. This can be attributed to differential
expansion and distortion due to the material difference.
Small variation can be observed between the stress at the top
and stress at the bottom. The distance is measured in meters.
To study the effect of clad layer thickness of residual stress
formation, the analysis is continued with various thickness.
4.2 Analysis of the Residual Stresses due to
Thickness of the Clad Material:
Analysis is carried out by varying the thickness of
the clad layer. Initially 1mm thickness is considered to study
the residual stress in the base structure.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
8www.ijert.org
IJERT
Fig. 4.20: Residual stress in the structure
Fig. 4.21: Residual stress due to 2mm thick clad material
The figure 4.20 shows residual stress formation of
74Mpa in the base material. This stress is less than 4mm clad
thickness. This can be attributed to lesser temperature effect
on the base structure.
The figure 4.21 shows residual stress formation of
78.2Mpa in the base material. This stress is less than 4mm
clad thickness but higher than 1mm thick cladding. This can
be attributed to higher thermal effect on the structure.
Fig. 4.22: Residual stress due to 3mm thick clad material
Fig. 4.23: Thickness Vs Vonmises Stress with clad
thickness
The figure 4.22 shows residual stress formation of
82.7Mpa in the base material. This stress is less than 4mm
clad thickness but higher than 1mm and 2mm thick cladding.
But the residual stress pattern is similar to the previous cases.
Table 4.1: Clad Thickness to Residual Stress formation
Clad Thickness Vonmises Stress (Mpa)
1 74
2 78.2
3 82.7
4 86.2
The table 4.1 shows vonmises stress due to varying
thickness of the clad material. The stress increasing with
thickness of the clad material. Almost uniform increase of
stress can be observed with clad thickness. This can be
attributed higher heat content deposited in the process.
The figure 4.23 shows variation of vonmises stress
with thickness of the clad material. The Vonmises stress is
uniformly increasing with thickness. In the graph, the X-axis
is represented with thickness of the clad material and Y-axis
is represented with Vonmises with MPa. Further analysis is
carried out with different materials to find best clad material.
Aluminum brass and Zerconium is considered for
comparision. The clad material properties are changed and
analysis is carried out to find residual stress formation. The
results are as follows.
4.3 Analysis of the Residual Stresses with General
Cladding Materials
Fig. 4.24: Residual stress with Aluminum Cladding
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
9www.ijert.org
IJERT
Fig. 4.25: Vonmises stress plot
The figure 4.24 shows residual stress with
aluminium cladding. Maximum stress is around 147Mpa.
This stress more than the first case. This can be attributed to
higher difference of thermal expansion coefficient of base
metal and cladding material. Thermal strain is directly
proportional to thermal expansion coefficient. Due to higher
deformation of clad metal and lower expansion of base
metal, the stresses will be more.
The figure 4.25 shows vonmises stress plot across
the geometry. Minimum stress is observed on the aluminium
material as the young’s modulus is much smaller than the
base metal modulus of rigidity.
Fig. 4.26: Residual stress with Brass Cladding
Fig. 4.27: Stress graph for Brass
The figure 4.26 shows residual stress with brass
cladding. Maximum stress is around 130Mpa. This stress
more than the first case. This can be attributed to higher
difference of thermal expansion coefficient of base metal
(11.7e-6) and cladding material (Brass -21e-6). Minimum
stress is observed on the cladding material as the young’s
modulus of Brass (103GPa) is almost half of the parent metal
(206GPa).
The figure 4.27 shows vonmises stress in the brass
cladding. Again the stresses are less in Brass material
compared to the base material. This is mainly due to higher
young’s modulus of steel compared to the brass. Also due to
higher difference of thermal expansion coefficients, the stress
generation is more in the structure.
Zirconium cladding
Zirconium is the best material for the cladding as it
comprises lowest thermal expansion coefficient compared to
the most of the engineering materials with goo mechanical
properties. The analysis is carried out by clad material
properties to zirconium. The analysis results are as follows.
Fig. 4.28: Residual stress with Zirconium cladding
Fig. 4.29: Residual stress in the zirconium
The figure 4.28 shows residual stress formation
with zirconium cladding. The least stress of 22.1Mpa can be
observed with Zirconium material. The stress patterns are
similar to the previous cases. But the stress generation is
least with zirconium cladding for the base material. This is
mainly attributed to the lowest coefficient of expansion of
zirconium.
The figure 4.29 shows residual stress in the
zirconium. The maximum stress of 8.69 Mpa can be
observed in the material. This is the lowest thermal residual
stress for the discussed materials. This results indicates
lowest distortion in the material. The maximum stresses are
observed at the central location shown with red colour.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
10www.ijert.org
IJERT
Fig. 4.30: Graphical plot of Residual stress
The figure 4.30 shows residual stress in the
structure with zirconium cladding. The maximum stress is
observed in the base metal and minimum stresses on
Zirconium. This is mainly due to difference in Young’s
modulus and thermal expansion coefficients.
Table 4.2: Residual stress generation in the base metal
with different cladding materials
Material Residual Stress(MPa)
Steel 86.2
Aluminium 147
Brass 130
Zirconium 22.1
The table shows residual stress formation with
different cladding materials. Zirconium shows minimum
residual stress in the structure. This can mainly attributed to
lower thermal expansion coefficient due to heating which
reduces the stresses in the structure.
4.4 Discussion:
In the present work cladding process is simulated
using Finite element analysis using ANSYS. Initially clad
geometry and base metal are modeled and split to ease map
meshing. The meshed geometry is attributed with relevant
properties. Initially the whole body is heated to 170 0c.
Further analysis is carried out with cladding simulation block
by block. The temperature plots are represented. The top clad
geometry is subjected to higher temperature and the region
away from cladding process is subjected to minimum
temperature. The geometry is brought back to initial
temperature by 2000 seconds cooling time. The analysis is
converted to structural analysis by considering thermal loads
to structural conditions. The coupled field analysis results
represent a stress gradient with minimum stress on top and
maximum stress in the constraint region indicates developed
residual stress in the cladding process. The results show a
stress development of 86.2 MPa in the structure. Further
analysis is carried out to find the effect on thickness of
cladding material on the residual stress formation. The
analysis is carried out for 1mm, 2mm, 3mm and 4mm
thickness. The results show lesser residual stress with lesser
thickness of clad material. This may be attributed to lower
heat input to the overall structure. Further analysis is carried
out with different cladding materials. The results shows
higher thermal expansion coefficient materials create higher
stresses compared to the lower thermal expansion coefficient
materials. The zirconium with its lower thermal expansion is
the best engineering clad material with minimum residual
stress formation in the structure. Also young’s modulus plays
important role in extent of stress in the materials.
5. Conclusions
5.1 Conclusions:
Thermal cladding process is simulated using Finite
element software ANSYS. The temperature distribution in
cladding process, usage of element birth and death, effect of
clad material thickness and different clad materials in
residual stress formation are obtained. The overall simulation
is process as follows.
Initially clad geometry along with base material
geometry are built and split to ease brick meshing of the
structure(Generally brick mesh gives better results
compared to the free mesh )
Initially thermal boundary conditions are applied with
initial preheat temperature of 170 0c.The cladding
process is simulated by element birth and death feature
with Newton Raphson iterative technique.
Temperature distribution and temperature variation
across the section are plotted
The members are cooled to initial temperature and
residual estimations are carried out
The coupled field analysis results show residual stress
formation in the structure after cooling it to the room
temperature. The maximum stresses are observed at the
constraint region and less at the outer surface.
Further analysis results are obtained by varying clad
material thickness and results are obtained for residual
stress formation. The results indicate lower residual
stress with lesser thickness of the clad material. This
may attributed to lower heat content due to lesser
thickness of the clad material.
Further analysis is carried out with general clad
materials. The results are obtained for residual stresses
for all the materials. The results shows zirconium is the
best cladding material with lowest residual stresses in
the structure. The results also prove that thermal
expansion coefficient and Young’s modulus plays
important role in the residual stress formation.
References
[1] Heyn, E. and Bauer, "Measurement of Residual
Stresses in Cold Drawn Metals." Internationale
Zeitschrift fur Met alio graphie, Vol.1, pp. 16-
50.1911
[2] Mesnager, M. "Methods de Determination des
tensions existant dans unCylindre Circulare."
Compt. Rend., Vol. 169, pp. 1391-1393.1919
[3] Sachs, G. Z. "Evidence of Residual Stresses in
Rod and Tubes." Trans. ASME, Vol. 19, pp. 352-
357.1927
[4] Hayes, Thomas, J. Elements of Ordinance. John
Wiley & Sons, N.Y.1938
[5] Timoshenko, S., Theory of Elasticity, McGraw-
Hill Book Co.,. Inc., New ...1941
[6] A. Robertson. ... Contractions and Stresses in Butt
Welded Steel Plates (London, H.M.S.O., 1950.
[7] Demorest, D. J. A Study of Residual Stresses in
Flat Beams by Electropolishing Methods, Ohio
State University, OH.1950
[8] Horger, O. J. Residual Stresses • Handbook of
Experimental Stress Analysis, Edited by M.
Hetenyi. John Wiley & Sons, N.Y.1950
[9] Leeser, D. O. and Daane, R. A. "Experimental
Stress Analysis." Argonne National Laboratory,
Lemont, IL. pp. 203-208.1953.
[10] Dieter Jr. G. E.: Mechanical Metallurgy. McGraw-
Hill, p395, 1961.
[11] I. J. Kumar and D. Rajgopalan, “Thermal stresses
in hollow cylinder due to a sinusoidal surface
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
11www.ijert.org
IJERT
heating source”, Defense Science Laboratory,
Delhi, 1969, Volume 1(3), Pages 305 -319.
[12] R. Srinivasan, C.S. Hartley and R. Bandy,
“Residual Stress Determination in Inconel-600
Tubes Using Electro-Chemical Machining,” in
Novel Techniques in Metal Deformation Testing,
R.H. Wagoner, Editor, TMS/AIME, Warrendale,
Pennsylvania, pp 163-174 1983.
[13] J. Rasty, “Effect of Combined Corrosion and
Residual Stress on ..... Research and Development
Center, United Technologies, July 11-12, 1987,
[14] Rasty, J. and Hartley, C. S.. Experimental
Measurement of Residual Stresses in Nuclear Fuel
Cladding, Louisiana State University, Baton
Rouge, 1987
[15] P. Dupas and D. Moinereau, “Evaluation of
Cladding Residual Stresses in Clad Blocks by
Measurements and Numerical Simulations” JOURNAL DE PHYSIQUE IV Colloque C1,
supplement au Journal de Physique 111, Volume 6,
Javier 1996.
[16] Rolf Paschold, ESAB GmbH Solingen,
“Submerged Arc strip cladding of continuous
casting rollers using OK band 11.82 and OK flux
10.07, Svetsaren Nr 1., 17-19, 2001.
[17] G. Sánchez Sarmiento, M.J. Mizdrahi, P. Bastias,
M. Pizzi, “Heat Transfer Thermal-Stress and Pipe-
whip Analysis in Steel Pipes of a Nuclear Power
plant”, ABAQUS Users’ Conference, Pages 631 –
645, 2004.
[18] Muhammad Abid, “Determination of safe
operating conditions for gasketed flange joint
under combined internal pressure and
temperature: A finite element approach”,
International Journal of Pressure Vessels and
Piping volume 83, Pages 433–441, January 2006.
[19] Iradj Sattari – Far, Magnus Andersson, “Cladding
Effects on Structural Integrity of Nuclear
Components”, Inspecta Technology AB. June
2006.
[20] Murali Krishna M, Shunmugam M.S., Siva Prasad
N, “A study on the sealing performance of bolted
flange joints with gaskets using finite element
analysis”, International Journal of Pressure Vessels
and Piping, Volume 84, February 2007, Pages
349–357, February 2007.
[21] Mohammad A. Irfan, Walter Chapman, “Thermal
stresses in radiant tubes due to axial,
circumferential and radial temperature
distributions”, Applied Thermal Engineering, page
1913-1920, Volume 29, September 2008,
[22] ANSYS analysis user’s manual, Version 10, theory
reference.
[23] Lochan Sharma, “Development of Submerged arc
welding fluxes for enhanced corrosion resistance of
structural steel welds”.
[24] “Technical handbook strip cladding”, ESAB AB.
International Journal of Engineering Research & Technology (IJERT)
Vol. 1 Issue 8, October - 2012
ISSN: 2278-0181
12www.ijert.org
IJERT